Download presentation

1
Ferroelectrics Basic principles

2
Outline What is the origin of electrostatic effects from crystalline materials? How might one classify ferroelectrics? A tour of some examples of ferroelectric materials…

3
An overview Non-conducting materials may have a net electrostatic polarisation induced by an external electric field. Where the affects upon observable properties such as elastic, optical and thermal behaviour is large, these materials are termed ferroelectrics. To gain some understanding, we’ll start with a simple model…

4
A naïve picture

5
Energetics

6
A naïve picture

7
A naïve picture

8
A naïve picture

9
A naïve picture The local alignment of dipoles can exist over any length scale. Different regions may exist with different polarisation orientations: Call these “domains” in line with magnetic materials. In contrast with magnetism, domain walls are abrupt.

10
Applied field Suppose we now apply an electric field, horizontal in the figure. If it is of sufficient strength, the small ions will be able to overcome the barrier and dipoles will switch direction The dipoles are polarised by the applied field. Domain walls move.

11
**Polarisation vs. E-field**

Suppose we start with a material where there are many domains which are aligned randomly. What is the initial polarisation?

12
**Polarisation vs. E-field**

If we apply a small electric field, such that it is not able to switch domain alignments, then the material will behave as a normal dielectric: PE As E is increased, we start to flip domains and rapidly increase P. When all domains are switched, we reach saturation. What happens if the E-field is now removed?

13
**Polarisation vs. E-field**

The value at zero field is termed the remnant polarisation. The value of P extrapolated back from the saturation limit is the spontaneous polarisation. Reversal of the field will eventually remove all polarisation The field required is the coercive field. Further increasing the reverse field will completely reverse the polarisation, and so a hysteresis loop is formed…

14
**Polarisation hysteresis**

15
**Polarisation hysteresis**

16
**Polarisation hysteresis**

The essential feature of a ferroelectric is not that there is a spontaneous polarisation, but that the spontaneous polarisation can be reversed by the application of an electric field.

17
E Now, E is small enough for the applied field to reverse the direction of the dipoles, i.e. move the atoms within the crystal, what else might affect this change? What are the relative sized of E and kBT? What will happen if EkBT?

18
Curie temperature Above a critical temperature the spontaneous polarisation will be lost due to one of two effects: A change of structure such that there is a single minimum in the energy mid-way between sites The rate that the small ions hop is so high that on average there is no net polarisation

19
Curie temperature This temperature is termed the Curie temperature, Tc, in light of the analogy with the transition temperature between ferromagnetism and paramagnetism. Above the Curie temperature, ferroelectrics behave as non-polar dielectrics, sometimes termed a paraelectric phase. Some ferroelectrics do not have a Curie temperature – why might this be?

20
**Other temperature effects**

In addition to the change in spontaneous polarisation, temperature affects the dielectric constant of the material, normally defined as the rate of change of dielectric displacement with electric field. For ferroelectrics where there is a non-linear relationship between D and P, we use =(D/ E)E=0

21
**Other temperature effects**

In some ferroelectrics, the temperature dependence of can be reasonably accurately represented by the Curie-Weiss law: = 0+C/(T-T0) C is the Curie constant T0 is the Curie-Weiss temperature, which in general differs from the Curie temperature (Tc) Close to T0 becomes very large. In some ferroelectrics, Tc≈T0, and the phase transition is of second order. In others Tc is far from T0 and the phase transition is first order.

22
06/04/2017 Beyond the naïve model In the model, we have picked out pairs of atoms, and attributed point dipoles associated with the combination of their charges and separations. More realistically, each unit cell carries a dipole moment: d = ∫∫∫(r).r.dv 0 (r) is the charge density (inc. ions), the integral is with respect to an arbitrary origin, and d is independent of its choice. The definition allows the polarisation to be as influenced by distortions in the electron density as it is by displacements in the point-like ion sites.

23
**Crystallography and ferroelectrics**

The crystal classification of a material has immediate implications for ferroelectric effects There are 32 crystal classes 11 of them have a centre of symmetry (centrosymmetric) and cannot support ferroelectricity Of the remaining 21, the O-point group (432) also excludes ferroelectricity. The remaining 20 classes all exhibit the piezoelectric effect… T Th O Td Oh C4 S4 C4h D4 C4v D2d D4h D2 C2v D2h C2 Cs C2h C1 Ci C3 S6 D3 C3v D3d C6 C3h C6h D6 C6v D3h D6h

24
**Crystallography and ferroelectrics**

The crystal classification of a material has immediate implications for ferroelectric effects There are 32 crystal classes 11 of them have a centre of symmetry (centrosymmetric) and cannot support ferroelectricity Of the remaining 21, the O-point group (432) also excludes ferroelectricity. The remaining 20 classes all exhibit the piezoelectric effect… T Th O Td Oh C4 S4 C4h D4 C4v D2d D4h D2 C2v D2h C2 Cs C2h C1 Ci C3 S6 D3 C3v D3d C6 C3h C6h D6 C6v D3h D6h

25
**Crystallography and ferroelectrics**

The crystal classification of a material has immediate implications for ferroelectric effects There are 32 crystal classes 11 of them have a centre of symmetry (centrosymmetric) and cannot support ferroelectricity Of the remaining 21, the O-point group (432) also excludes ferroelectricity. The remaining 20 classes all exhibit the piezoelectric effect… T Th O Td Oh C4 S4 C4h D4 C4v D2d D4h D2 C2v D2h C2 Cs C2h C1 Ci C3 S6 D3 C3v D3d C6 C3h C6h D6 C6v D3h D6h

26
Piezoelectric effect The application of an electric field induces a geometrical change. Alternatively, a distortion of the material induces a potential difference. Used in many electrical devices, e.g. sound-to-electricity

27
**Crystallography and ferroelectrics**

The crystal classification of a material has immediate implications for ferroelectric effects There are 32 crystal classes 11 of them have a centre of symmetry (centrosymmetric) and cannot support ferroelectricity Of the remaining 21, the O-point group (432) also excludes ferroelectricity. The remaining 20 classes all exhibit the piezoelectric effect Of these, 10 have a unique polar direction. T Th O Td Oh C4 S4 C4h D4 C4v D2d D4h D2 C2v D2h C2 Cs C2h C1 Ci C3 S6 D3 C3v D3d C6 C3h C6h D6 C6v D3h D6h

28
**Crystallography and ferroelectrics**

Crystal classes with a unique polar axis are called polar. The spontaneous polarisation can be seen in terms of its change with temperature: the pyroelectric effect. The 10 polar classes are therefore sometimes referred to as the pyroelectric classes. Ferroelectric crystals must belong to the pyroelectric classes. But Ferroelectrics must exhibit the hysteresis, so we define ferroelectric crystals as pyroelectric crystals that exhibit reversible polarisation.

29
**Classification of ferroelectrics**

“Crystal-chemical”: hydrogen-bonded (e.g. KH2PO4) or otherwise (e.g. double oxides). No. of polarisation directions: single direction (e.g. PbTa2O6), several equivalent directions (e.g. BaTiO3). Centrosymmetric non-polar phase: E.g. Rochelle salts exhibit piezoelectric phase above Tc, whereas BaTiO3 is centrosymmetric. First vs. second order phase change at Tc. It turns out this corresponds to the value of the Curie constant (C), one group being of the order of 103K, and the other 105K. These four classifications do not necessarily coincide.

30
Antiferroelectrics Polar Antipolar

31
Antiferroelectrics If the free energy of an antipolar phase is comparable to the polar state then the material is termed antiferroelectric. If a material exhibits ferroelectric effects in one polar direction, and antiferroelectric effects perpendicular, it may be termed ferrielectric. Antipolar Polar

32
Perovskites Perovskite is a naturally occurring mineral with chemical formula CaTiO3. This is a prototype for many ABO3 materials which are very important in ferroelectrics. These materials may be envisaged by consideration of a non-polar, cubic basic building block…

33
Perovskites A O B

34
Perovskites Below the Curie temperature, these crystals undergo symmetry lowering distortions. We’ll initially focus up the distortions of BaTiO3. There are three phase transitions in order of decreasing temperature: 120oC, 5oC, and -90oC.

35
BaTiO3 Above 120oC BaTiO3 is cubic (non-polar) Ba O Ti

36
BaTiO3 From 120oC down to ~5oC, there is a distortion to a tetragonal phase. All of the cube directions can undergo this type of distortion: this leads to complexity in domain formation.

37
BaTiO3 From 5oC down to around -90oC the structure is orthorhombic by dilation along [110] directions and contraction along [1-10]. There are 12 possible orientations.

38
BaTiO3 Finally the lowest temperatures yield rhombohedra (distortions along the body diagonal). There are therefore 8 equivalent distortion directions

39
**PbTiO3 internal structure**

The foregoing analysis of BaTiO3 focuses on the shape of the unit cell. However, for the ferroelectric effect, we also require internal structural changes. In light of current interest in Cu-related defects in lead titanium tri-oxide, we’ll review this tetragonal system at room temperature…

40
**PbTiO3 internal structure**

X-ray and neutron scattering yield the internal structure: a=3.904Å, c=4.150Å, so that c/a=1.063. Taking the Pb site as the origin, the displacements are zTi=+0.040 zOI=+0.112 zOII=+0.112 Here OI are the polar O-sites, and OII are the equatorial. Thus, since the oxygen atoms are all displaced by the same amount, the oxygen cage remains intact, and shifts relative to the Ti and Pb sites.

41
PbTiO3 Ti O Pb

42
PbTiO3 It should be clear that this system has a net dipole in each unit cell, and furthermore that the distortion can be along any of the x, y and z directions. In real PbTiO3, there is a non-trivial role for point defects, especially O-vacancies.

43
Bibliography C. Kittel, “Introduction to Solid State Physics”, Wiley 1956. Franco Jona and G. Shirane, “Ferroelectric Crystals”, International Series of Monographs on Solid State Physics, Pergamon Press 1962.

Similar presentations

OK

14.1 Essential Questions What is the kinetic theory of matter?

14.1 Essential Questions What is the kinetic theory of matter?

© 2018 SlidePlayer.com Inc.

All rights reserved.

To ensure the functioning of the site, we use **cookies**. We share information about your activities on the site with our partners and Google partners: social networks and companies engaged in advertising and web analytics. For more information, see the Privacy Policy and Google Privacy & Terms.
Your consent to our cookies if you continue to use this website.

Ads by Google

3d backgrounds for ppt on social media Ppt online shopping project proposal Marketing mix ppt on airtel Ppt on wildlife conservation in india Ppt on water cycle for kindergarten Ppt on internet banking in india Ppt on any social issues in india Ppt on instrument landing system history Ppt on world ozone day Ppt on event driven programming in java